Impact of Thiocyanate Salts on Physical, Thermal, and Rheological Properties of Zein Films
Gordon W. Selling,1,2 Ashley Maness,1 Scott Bean,3 and Brennan Smith3
ABSTRACT Cereal Chem. 90(3):204–210
A new class of zein additives was investigated, thiocyanate salts. Am- differential scanning calorimetry. In zein films in which TEG was present, monium, potassium, guanidine (GTC), and magnesium thiocyanate salts these salts increased elongation and reduced tensile strength. However, were added to solutions of zein in with various amounts of tri(ethylene unlike traditional plasticizers (such as TEG), when the salts were used as glycol) (TEG), cast as films, and then tested to determine the impact that the only additive, elongation was not increased and tensile strength was each salt had on properties. The presence of these salts affected solution not decreased. Of the salts tested, GTC in combination with TEG was rheology and intrinsic viscosity, demonstrating that the salts interacted found to increase elongation the most. The impact of salts on elongation with the protein. It was found that these salts acted as plasticizers, as they was greatly affected by the relative humidity in which the samples were lowered the glass transition temperature of zein when evaluated with stored.
With the production of ethanol from corn, whether production (salt out, kosmotropes, to the left in Fig. 1) (Whitford 2005; Cho is done with dry- or wet-milling processes, a great deal of pro- et al 2008; Rembert et al 2012). teinaceous coproduct is generated (Lawton 2002). The dominant Inorganic salts are known to interact with proteins, altering the protein present in the dry- or wet-milling coproduct is zein. De- protein structure or changing their solubility characteristics (Bald- veloping improved end uses for zein will improve the economics win 1996). Salts such as calcium chloride and sulfate have been of the ethanol production industry. In the early 1930s, zein was shown to alter the physical properties of soy protein films through used in the textile fiber market as a wool alternative (Swallen the cation by apparently forming calcium bridges between proteins 1939; Croston et al 1945; Evans and Croston 1949). For use in (Park et al 2001). However, calcium cations and chloride anions are this market, the zein was treated with formaldehyde to impart known to increase its solubility, whereas sulfate anions will de- improved physical properties and solvent durability. With the crease its solubility. Sodium lactate was shown to reduce tensile introduction of textile fibers based on petroleum feeds, the use strength and increase elongation of whey protein films (Zinoviadou of zein in the textile fiber market disappeared. To replace prod- et al 2010); however, in that study only the one salt was evaluated, ucts that use nonrenewable materials, zein products need im- and both the sodium and lactate ions would be in the middle of the proved elongation and improved solvent resistance. Various non- Hofmeister series in terms of their impact on a protein. Salts have formaldehyde routes have been investigated to improve the solvent also been used to modify the properties of zein. Alkali salts typi- resistance of zein, including glyoxal (Selling et al 2012), glu- cally having long-chain fatty acid anions have been shown to alter taraldehyde (Sessa et al 2008), multivalent (e.g., citric) acids the solubility of zein (James 1945). However, these long-chain fatty (Reddy et al 2009; Jiang and Yang 2011), and diisocyanates (Wu acids have been shown to have compatibility issues with zein (San- et al 2003; Yao et al 2007). These reagents typically lead to tosa and Padua 2000). Other researchers have used salts such as branching and/or cross-linking and lower elongation. Tech- sodium chloride, sodium sulfate, zinc sulfate, ammonium sulfate, niques have been developed to improve the elongation of zein, ammonium phosphate, and so on to modify the properties of zein albeit with reduced tensile strength, but these techniques typi- cross-linked with formaldehyde (Cline 1949; Croston and Evans cally involve the use of plasticizers such as diols, triols, and 1949; Jenkins and Magee 1958). In these studies, the impact of long-chain carboxylic acids (Padua and Santosa 1999; Para- salts was not detailed in a controlled fashion, nor were the singular mawati et al 2001; Lawton 2004; Gao et al 2006; Ghanbarzadeh impacts of the salts on zein properties determined. Ammonium et al 2007; Gillgren and Stading 2008; Gillgren et al 2009; Wu thiocyanate (ATC) has been used in conjunction with p-toluenesul- et al 2010). These additives suffer from moisture sensitivity, fonic acid, monochloroacetic acid, and formaldehyde to provide migration, and loss of plasticizer resulting from deposit forma- durable zein fibers (Huppert 1946). It was proposed in a patent by tion or volatility. There is a need for developing additional Huppert (1946) that the purpose of the ATC was to convert the methods to improve the elongation of zein. globular zein protein into a fibrous structure; however, no data was The Hofmeister series (abbreviated listing in Fig. 1) is a set of provided to support this claim. A systematic study with salts that fit guidelines that can be used to determine if a particular salt will the series has not been undertaken. increase protein solubility in water (salt in, chaotropes, to the The effect that Hofmeister salts have on proteins has almost right in Fig. 1) or cause a protein to decrease in solubility in water exclusively been studied in water. With zein not being soluble in water, it is not clear what effect these salts will have on zein. The salts in this series have been evaluated in conjunction with 1 Plant Polymer Research Unit, National Center for Agricultural Utilization Re- polymers other than proteins (Heuvingh et al 2005), albeit in search, USDA–Agricultural Research Service, 1815 N. University St., Peoria, IL 61604. Mention of trade names or commercial products in this publication is water solution. Thiocyanate salts have been used in zein systems solely for the purpose of providing specific information and does not imply rec- (Huppert 1946), and based on the Hofmeister series, the thiocya- ommendation or endorsement by the USDA to the exclusion of others that may also be suitable. USDA is an equal opportunity provider and employer. 2 Corresponding author. Phone: (309) 681-6337. Fax: (309) 681-6691. E-mail: [email protected] 3 USDA–Agricultural Research Service CGAHR, 1515 College Ave., Manhattan, KS 66502. http://dx.doi.org/10.1094/ CCHEM-09-12-0123-R This article is in the public domain and not copyrightable. It may be freely re- printed with customary crediting of the source. AACC International, Inc., 2013. Fig. 1. Abbreviated Hofmeister series.
204 CEREAL CHEMISTRY nate anion is among the strongest anions for impacting the prop- added, and then the solution was stirred for 1 hr. For example, if erties of a protein in water. Although typically the anion has a the sample was to be composed of zein having 17.5% TEG, then larger effect on protein solubility in water systems (Rembert et al 1.86 g of TEG would be added to 27 g of 90% EtOH/water, and 2012), the cation, as detailed earlier involving calcium ions, can then 8.75 g of zein would be added. For salt formulations after the play a role as well. In addition, many of these protein–salt studies addition of TEG and the 2 min of stirring, the salt was added. were performed in solution; it is not clear whether the cation or After the salt had completely dissolved, the zein was added to the anion will have a larger effect on a protein in the solid state. Se- solution, followed by stirring for 1 hr. For example, if the sample lect thiocyanate salts can be found that are soluble in 90% etha- was to be composed of zein having 17.5% TEG and 8% ATC, nol/water. If thiocyanate changes the structure of a protein while then 2.06 g of TEG was added to 27 g of 90% EtOH/water, and in solution, then the structure that the protein has while drying then 0.94 g of ATC was added. After dissolution, 8.75 g of zein may be different relative to the control and perhaps give increased was added. For one formulation (sample 8-ATC-17.5 31.3%), elongation. Although the cation may have a lesser role on protein which was used for rheological testing only, the amount of 90% properties per the Hofmeister series, it is not clear how cation EtOH/water used was 25.80 g so as to increase the relative selection will impact zein properties. To define the impact that amount of zein for solution rheological testing. The zein solutions thiocyanate salts have on zein, various thiocyanate salts were in- were then degassed under vacuum, poured into a gasket mold, and corporated into zein solutions. Cations were selected to provide allowed to dry in a chemical hood for a week. The mold was a solubility in the solvent used, as well as to allow the investigation rubber gasket having an opening in the center with dimensions of of protein–cation interactions according to the Hofmeister series. approximately 13 × 26 cm that was placed on a Teflon-coated Investigations in which the anion is varied are in progress and will glass plate. After three days, the rubber gasket was removed, and be reported at a later date. The zein thiocyanate salt formulations the film was carefully lifted up and turned over to help the film to had some of their solution properties characterized, and then films dry completely. were cast, dried, and characterized. Sample Evaluation MATERIALS AND METHODS Tensile property samples were stored at 23°C and 15, 50, and 70% rh for five days before testing physical properties. TS, YM, Materials and Equipment and %Elo data are presented as the calculated means and stand- Zein was obtained from Freeman Industries (Tuckahoe, NY, ard deviations for a minimum of five samples. The model that U.S.A.), lot #40006124 (14.4% nitrogen, 4.8% moisture). Ethyl was used to predict TS versus total plasticizer present was devel- alcohol (EtOH, Sigma-Aldrich, Saint Louis, MO, U.S.A.) and oped on Minitab 15 (Minitab, State College, PA, U.S.A.). The 1H deionized water were used to generate the solvent in which the NMR spectra were obtained after dissolution in 90% ethanol- zein and salts were dissolved. Tri(ethylene glycol) (TEG) was d6/10% deuterium oxide at room temperature with and without used as received from Sigma-Aldrich. Ammonium (ATC), po- the addition of TEG. Intrinsic viscosity (η) measurements were tassium (KTC), guanidine (GTC), and magnesium thiocyanate made with a Schott AVS 360 injection pump, CT 52 water bath (MTC) salts were obtained from J. T. Baker Chemical (Austin, (set to 30°C), Dilut4 controlling software, and Schott 53110 cap- TX, U.S.A.), Sigma-Aldrich, Sigma-Aldrich, and Pfaltz and Bauer illary viscometer tube (Schott Instruments, College Station, TX, (Waterbury, CT, U.S.A.), respectively. Sample thicknesses of cast U.S.A.). Intrinsic viscosity solutions were prepared as follows: to films were measured at five different locations with a micrometer 30 g of sample was added 100 mL of 90% EtOH/water; it was (model 49-63, Testing Machines, Amityville, NY, U.S.A.). Con- then stirred for 1 hr at room temperature and filtered through a stant relative humidity (50 and 70% rh) at 23°C was obtained by Whatman nylon 0.45 micron syringe filter. A sample of filtered storing samples in a constant temperature and humidity room. solution was used to determine concentration by drying over- Constant relative humidity of 15% rh at 23°C was obtained with a night at room temperature and then in an oven at 120°C over- saturated lithium chloride solution and a desiccator stored in the night. Filtered solution (15 mL) was used in the intrinsic viscos- constant temperature room. Moisture contents were measured ity instrument, for which five time measurements were made on with an Ohaus MR45 moisture analyzer at 105°C for 20 min on each solution. Five dilutions were then automatically made (ad- 1 g of sample. Tensile strength (MPa, TS), Young’s modulus dition of 5, 5, 5, 7, and 9 mL), for which a time measurement (MPa, YM), elongation to break (%Elo), and toughness (MPa) was made after addition of each aliquot of 90% EtOH/water. were evaluated for each sample with an Instron universal testing From the intrinsic viscosity values, the radius of gyration and machine model 4201 and an ASTM D638 type V test. Physical mean end-to-end distance could be calculated (Seymour and properties were determined with a crosshead speed of 10 mm/min, Carraher 1992). The DSC scans were conducted on samples that a gauge length of 7.62 mm, and either a 1 kN load cell or a 100 N had been stored at 50% rh for five days to minimize the effects of load cell, depending on the strength of the samples. Toughness moisture. The samples were run through two cycles on the DSC: was determined by dividing the energy to break by the volume of first from –88 to 160°C, then back to –88°C, and finally up to the sample (gauge length × width × depth). Toughness would be 270°C. The DSC traces reported were from the second heating analogous to the area underneath the stress–strain curve. NMR cycle. Solution rheology studies in which the strain rate was var- spectra were run on a Bruker 500 MHz NMR (Billerica, MA, ied from 1 to 100 sec–1 were averaged to obtain the viscosity of U.S.A.) in 90% ethanol-d6/10% deuterium oxide (Cambridge these Newtonian zein solutions. The geometry used for these Isotope, Andover, MA, U.S.A.). Differential scanning calorimetry viscosity measurements was a 50 mm titanium cone and plate (DSC) was performed to determine the glass transition tempera- with a 0.046 mm gap and an angle of 0.0401 rad. The tempera- tures of zein control films, zein/TEG control films, and zein/TEG/ ture was controlled via a Peltier plate at a temperature of 25 ± thiocyanate salt films using a TA Instruments model Q2000 DSC 0.1°C, and a humidity cover was used to prevent solution evapo- (New Castle, DE, U.S.A.). Solution rheology experiments were ration. Zein films with dimensions of 0.3–0.4 mm thickness, 5– done on a TA Instruments ARES LS-1 controlled strain rheometer. 10 mm width, and 10–15 mm length, depending on the zein films Dynamic mechanical analyses (DMA) were performed with a TA provided, were submitted for DMA analyses. Dynamic tempera- Instruments ARES LS-2 controlled strain rheometer. ture ramps were run on these films from 25 to 200°C at 1°C/min with a strain of 0.5% and a frequency of 1 rad/sec. A constant Solution Preparation normal force of 0 ± 10 g was placed on the sample as it was To 27 g of 90% EtOH/10% water (m/m; hereafter 90% EtOH/ heated; in this fashion, if the sample expanded or contracted dur- water) was added the TEG. After 2 min of stirring, the zein was ing the analysis, it could be monitored. Some samples when
Vol. 90, No. 3, 2013 205 heated to temperatures above 140°C would fail before reaching ously that the addition of salts can affect the solution rheological final temperature (200°C). properties of polyamides (Shashkina et al 2005), and it was of interest to determine if the thiocyanate salts being studied here RESULTS AND DISCUSSION affected the rheology of zein in solution. Three solutions were prepared, C17.5, 8-ATC-17.5, and 8-ATC-17.5 31.3%. In sample Shown in Table I are the zein formulations tested in this work. 8-ATC-17.5 31.3%, the total solvent was adjusted so that the Included is a column detailing the total amount of plasticizer (in overall protein % solids was the same as the control. This was mol/kg of zein) present in the sample, which makes it easier for done because the salt being added may act as a diluent, and if the comparisons between samples. Based on DSC and DMA analysis viscosity was reduced (with the addition of 8% ATC, the % pro- discussed later, the thiocyanate salts were found to be plasticizers tein solids was 22.6 instead of 23.3%), it may have been because for zein. To make a good comparison on the effectiveness of these the amount of protein was reduced. Shown in Figure 2 is the vis- thiocyanate salts to plasticize zein, a known zein plasticizer, TEG cosity of these solutions versus shear rate. With the addition of the (Lawton 2004; Selling et al 2004), was used as an additional con- salt, there was a modest reduction in viscosity. This reduction was trol. Various amounts of TEG were used to establish trends. These still observed when the % protein solids of the solution was in- were coded as samples C0–C30, for which the C represents con- creased to match that of the control. This observation suggested trol and the number represents the amount of TEG (in % of the that there was an interaction between the protein and the salt. amount of zein) used in that sample. For example, formulation With the observed differences in solution rheology, intrinsic C17.5 was a sample made from zein and sufficient TEG to give viscosity studies were also undertaken. To perform intrinsic vis- 17.5% in the sample. Five levels of ATC were evaluated with cosity, it is important that the overall % solids be known. This 17.5% TEG used as a coplasticizer. In addition, one level of ATC, value is typically determined with oven drying. Given that TEG is 4%, was evaluated with various amounts of TEG to determine if somewhat volatile, it was not used in this study, as it would intro- synergism was present. For example, formulation 4-ATC-17.5 duce error in the solids measurements. The intrinsic viscosity of was a sample made from zein, ATC, and TEG to give a sample zein in 90% EtOH/water was determined to be 0.147 dL/g (stand- having 4% ATC and 17.5% TEG. Additional thiocyanate salts, ard deviation = 0.007 dL/g). For the sample having 8% ATC, the KTC (K+ is kosmotropic), GTC (guanidinium ion is very chao- intrinsic viscosity was 0.168 dL/g (standard deviation 0.011 tropic), and MTC (Mg+2 is chaotropic), were evaluated at single dL/g). These results suggested that in the presence of ATC, the levels of TEG. When evaluating MTC it was understood that in zein protein opened up, leading to a higher mean end-to-end dis- addition to it having a different cation, the cation also had a tance and a higher radius of gyration. The mean end-to-end dis- charge of +2. Also, because of the rather limited number of vola- tance and radius of gyration were, respectively, 115.5 and 47.1 Å tile solvents that zein is soluble in, the choice of potential salts for the control and 120.7 and 49.3 Å for the sample having 8% was also somewhat limited, as salts could only be chosen if they ATC. Both the intrinsic viscosity and solution rheology results were soluble in the same solvent used to dissolve the protein zein. suggested that ATC interacted with the zein protein. All films were of good quality with no obvious defects. 1H NMR Solution Rheology and Intrinsic Viscosity Although infrared spectroscopy (IR) can be used to discern A brief study was undertaken to determine if these types of changes in protein structure, for the films made here, spectral salts had a large impact on the structure of zein in solution, as changes (beyond addition of the S=C=N stretch in the IR spectra determined with rheological techniques. It has been shown previ- with added ATC) were not observed with the addition of the thio-
TABLE I Zein–Thiocyanate Salt Formulations Zein TEG TEG Salt Salt Total Plasticizer Formulation (g) % TEG (g) (mol/kg of zein) Salt % Salt (g) (mol/kg of zein) (mol/kg of zein) C0 8.75 0.0 0.00 0.00 … … … … 0.00 C5 8.75 5.0 0.46 0.35 … … … … 0.35 C10 8.75 10.0 0.97 0.74 … … … … 0.74 C13 8.75 13.0 1.31 1.00 … … … … 1.00 C15 8.75 15.0 1.54 1.18 … … … … 1.18 C17.5 8.75 17.5 1.86 1.41 … … … … 1.41 C20 8.75 20.0 2.19 1.66 … … … … 1.66 C25 8.75 25.0 2.92 2.22 … … … … 2.22 C30 8.75 30.0 3.75 2.85 … … … … 2.85 0.5-ATC-17.5 8.75 17.5 1.87 1.42 ATC 0.5 0.05 0.08 1.50 1-ATC-17.5 8.75 17.5 1.88 1.43 ATC 1.0 0.11 0.16 1.59 2-ATC-17.5 8.75 17.5 1.90 1.45 ATC 2.0 0.22 0.33 1.77 4-ATC-17.5 8.75 17.5 1.95 1.48 ATC 4.0 0.45 0.66 2.14 8-ATC-17.5 8.75 17.5 2.06 1.56 ATC 8.0 0.94 1.41 2.97 8-ATC-17.5 31.3%a 8.75 17.5 2.06 1.56 ATC 8.0 0.94 1.41 2.97 4-ATC-0 8.75 0.0 0.00 0.00 ATC 4.0 0.36 0.55 0.55 4-ATC-2.5 8.75 2.5 0.23 0.18 ATC 4.0 0.37 0.56 0.74 4-ATC-5 8.75 5.0 0.48 0.37 ATC 4.0 0.38 0.58 0.94 4-ATC-10 8.75 10.0 1.02 0.77 ATC 4.0 0.41 0.61 1.39 4-ATC-13 8.75 13.0 1.37 1.04 ATC 4.0 0.42 0.63 1.68 4-ATC-15 8.75 15.0 1.62 1.23 ATC 4.0 0.43 0.65 1.88 4-ATC-17.5 8.75 17.5 1.95 1.48 ATC 4.0 0.45 0.67 2.15 6-GTC-17.5 8.75 17.5 2.00 1.52 GTC 6.0 0.69 0.66 2.18 5-KTC-17.5 8.75 17.5 1.98 1.50 KTC 5.0 0.56 0.66 2.16 7-MTC-17.5 8.75 17.5 2.03 1.54 MTC 7.0 0.81 0.66 2.20 a Used 25.8 g of 90% EtOH/water. TEG = tri(ethylene glycol); ATC = ammonium thiocyanate; GTC = guanidine thiocyanate; KTC = potassium thiocyanate; and MTC = magnesium thiocyanate.
206 CEREAL CHEMISTRY cyanate salts (data not shown). Protein structural changes have Lamsal 2011), it was not surprising that the peaks were broad. On been observed with NMR (Tamiola and Mulder 2012). To deter- examination of these two spectra, it could be noted that the shape mine if the addition of these salts altered the structure of zein, of the peak in this region changed with the addition of ATC. This NMR spectroscopy was employed. Shown in Figure 3 are the observation suggested that the environment around these hydro- NMR spectra for zein with 17.5% TEG (Fig. 3A) and zein, 8% gen atoms changed because of the presence of the salt. The im- ATC, and 17.5% TEG (Fig. 3B). The overall solids were reduced pact of thiocyanate salts on the NMR spectra of proteins has been so that the viscosity of the solution was such as to make obtaining studied previously, and it was found to change the position of the NMR spectra possible. The peaks located between 4.3 and 5.7 methylene protons on the protein backbone (Rembert et al 2012). were different for the two samples (Fig. 3). Spectra of TEG with and without ATC were also run. The peaks for the CH2 groups α DSC and DMA to the oxygens were unchanged with the addition of ATC to the A standard method for determining if a polymer additive is a TEG, showing that the differences observed were not because of plasticizer is through the use of DSC (Lawton 2004). Shown in TEG/ATC interaction (data not shown). In addition, zein and Figure 4 are the DSC traces for C0, C17.5, 8-ATC-0, and 8-ATC- zein/ATC spectra were also obtained without TEG, and the same pattern was observed (data not shown). The peaks at 3.6 and 3.7 resulted from the added TEG as well as residual protio peaks for the NMR solvent (CD3CD2OD). There, sharpness was because as small molecules they would freely rotate in the solvent and the peaks would not be broadened. Peaks located between 4.3 and 5.7 are typically attributed to hydrogen atoms on carbon that are α to electron-withdrawing groups such as hydroxyl (Silverstein et al 1981). Given that zein is a mixture of proteins (Paraman and
Fig. 4. Differential scanning calorimetry trace of C0, C17.5, 8-ATC-17.5, and 8-ATC-0. X indicates the Tg of the respective samples.
Fig. 2. Viscosity of select zein solutions at various shear rates, = C17.5; = 8-ATC-17.5; and = 8-ATC-17.5 31.3%.
Fig. 3. 1H NMR spectra. A, zein with 17.5% tri(ethylene glycol) (TEG); Fig. 5. Dynamic mechanical analysis scans of C17.5 and 8-ATC-17.5 and B, zein, 8% ammonium thiocyanate, and 17.5% TEG. from –50 to 100°C. Sample 8-ATC-17.5 failed at 60°C.
Vol. 90, No. 3, 2013 207 17.5. With the addition of TEG or ATC, the Tg decreased (X in the control at all temperatures. This result was to be expected for a figure indicates the Tg) from 67°C for the control to 37, 58, and plasticizer. The G″ of the ATC sample was more similar to the 30°C, respectively. The lowest Tg was for the sample having both control at very low temperatures. Above –5°C, G″ of 8-ATC-17.5 additives. This same trend was observed for the other salts; with began to decline rapidly. When the temperature reached 60°C, the the addition of more or less ATC, the Tg increased or decreased, 8-ATC-17.5 sample failed. Shown in Table II are the G′ and G″ respectively. values for select samples at 40°C. It is interesting to note that at To complement DSC, DMA is often used. In this technique, the low levels of ATC, the modulus was actually higher than the con- sample is flexed at a defined strain with varying temperature trol at 40°C. Over 2% ATC was required for the G′ and G″ to be while the stress is monitored. From these measurements, the elas- lower than the control’s G′ and G″. At 4 and 8% ATC, G′ and G″ tic modulus (G′) and viscous modulus (G″) can be measured. Fig- were much lower than the control’s G′ and G″. ure 5 shows the DMA traces for C17.5 and 8-ATC-17.5 from –50 to 100°C. G′ for the samples with ATC was lower than that of the Physical Properties—ATC Shown in Table III are the physical properties of films after storing at 50% rh. For the ATC salt, two sets of results are shown: TABLE II ′ ″ using variable amounts (0.5–8%) of ATC at the same % of TEG G and G for Select Formulations at 40°C (17.5%) and using 4% ATC with variable amounts of TEG (0– Sample G′ (MPa) G″ (MPa) 17.5%). In examining the series of samples with various amounts C17.5 223 51 of ATC (##-ATC-17.5), it could be seen that as the amount of 0.5-ATC-17.5 553 69 ATC increased, %Elo increased and TS and YM decreased, dem- 1-ATC-17.5 492 96 onstrating that it affected physical properties like a plasticizer. In 2-ATC-17.5 398 92 the series in which the amount of ATC was fixed at 4% and the 4-ATC-17.5 83 31 amount of TEG varied, it could be observed that ATC was not an 8-ATC-17.5 28 14 effective plasticizer when used on its own. When 4% ATC was the
TABLE III Physical Properties of Zein Films with Various Amounts of TEG and Thiocyanate Salts, Stored at 50% rha Total Plasticizer TS %Elo YM Toughness Formulation (mol/kg of zein) TS (St. Dev.) %Elo (St. Dev.) YM (St. Dev.) Toughness (St. Dev.) C0 0.00 30.7 0.8 6.7 0.2 595 8 1.1 0.0 C5 0.35 25.9 1.1 5.6 0.5 527 12 0.8 0.1 C10 0.74 24.8 1.1 5.6 0.5 527 12 0.8 0.1 C13 1.00 23.9 1.1 7.7 0.7 404 19 0.9 0.1 C15 1.18 19.9 1.2 10 1 295 8 1.1 0.3 C17.5 1.41 10.2 0.7 52 12 120 11 2.9 0.3 C20 1.66 4.6 0.3 286 17 36 3 10.0 0.4 C25 2.22 1.2 0.1 980 26 2 1 8.4 0.4 C30 2.85 0.5 0.0 1,048 35 0 0 3.2 0.2 0.5-ATC-17.5 1.50 10.1 0.5 85 19 100 4 6.3 1.2 1-ATC-17.5 1.59 8.4 0.5 101 17 78 6 6.5 1.0 2-ATC-17.5 1.77 4.2 0.1 223 74 37 4 8.1 2.5 4-ATC-17.5 2.14 1.6 0.1 499 54 7 1 7.1 0.7 8-ATC-17.5 2.97 0.1 0.0 3,368 126 0 0 1.6 0.5 4-ATC-0 0.55 27.1 2.1 6.8 0.3 515 42 0.9 0.0 4-ATC-2.5 0.74 24.2 0.6 6.3 1.3 484 13 0.8 0.3 4-ATC-5 0.94 23.8 1.1 13 2 392 19 1.9 0.4 4-ATC-10 1.39 16.6 0.8 28 4 205 16 3.5 0.4 4-ATC-13 1.68 9.6 0.6 71 5 107 8 4.4 0.7 4-ATC-15 1.88 5.8 0.1 169 10 51 4 8.3 0.6 4-ATC-17.5 2.15 1.6 0.1 499 54 7 1 7.1 0.7 6-GTC-17.5 2.18 0.7 0.1 1,203 91 2 0 7.3 1.2 5-KTC-17.5 2.16 1.1 0.0 879 11 9 6 6.6 0.7 7-MTC-17.5 2.20 2.2 0.4 399 56 13 4 8.2 1.7 a TEG = tri(ethylene glycol); TS = tensile strength; %Elo = elongation to break; YM = Young’s modulus; ATC = ammonium thiocyanate; GTC = guanidine thio- cyanate; KTC = potassium thiocyanate; and MTC = magnesium thiocyanate.
Fig. 6. A, Elongation to break (%Elo) versus total plasticizer; and B, toughness versus total plasticizer.
208 CEREAL CHEMISTRY only additive, the %Elo was the same as the control for which no each plasticizer versus TS (Fig. 7). The experimental results could plasticizer was present. Between 5 and 10% TEG was needed be placed into a model developed through Minitab 15, in which before an effect on %Elo was observed. Apparently, the ATC was the two additives as well as their cross-term were selected for the not capable of interacting with the protein in the solid state to the model. Given that a certain amount of TEG was needed for the extent needed without the presence of an additional plasticizer to ATC to impact properties, the cross-term was chosen as well. In allow increased polymer chain mobility. Therefore, ATC did not this model, as expected, both TEG and ATC reduced TS. The pre- function in the role of a classic plasticizer, and it did depress the dicted TSs agreed fairly well (R2 = 0.89) with those observed Tg of the protein; physical properties were little changed when it experimentally. In this way, a given TS could be achieved through was used alone. A number of TEG controls (C0–C30) were also using various amounts of each plasticizer. prepared to better gauge the effects of ATC as a plasticizer. These samples clearly demonstrated the effect of increasing plasticizer; Effect of Cation Selection as the level of TEG was increased from 0% TEG (C0) to 30% Although the anion may typically have a larger effect on pro- TEG (C30), TS and YM decreased and %Elo increased. When the teins, the cation can play a role as well (Heuvingh et al 2005; total amount of plasticizer (measured in moles of plasticizer per Whitford 2005). To define what impact changes in cation have on kilogram of material) was plotted versus %Elo (Fig. 6A), it could the protein, other thiocyanate salts were tested. Based on protein be seen that at lower levels of plasticizer, TEG alone provided solubility in water-based systems, the ammonium salt tested higher %Elo. At the higher levels of plasticizer when TEG and (ATC) should destabilize the zein in solution. The remaining salts ATC were used, the combination of plasticizers gave a higher would begin to stabilize the protein, and the order of increasing %Elo. Toughness is a measure of the area underneath a stress– stability would be the potassium salt (KTC), the magnesium salt strain curve. When toughness was plotted against total plasticizer (MTC), and finally the guanidinium salt (GTC). The GTC would content (Fig. 6B), it could be seen that at lower levels of ATC, the stabilize the zein to the largest extent in a water solution if the toughness was improved relative to the use of TEG alone. An Hofmeister series trends can be applied here. Films containing interesting trend was observed when examining the amount of these salts were produced and their physical properties evaluated. When compared with ATC (Table III), GTC (tested in 6-GTC- 17.5) had higher %Elo and lower TS. The impact KTC (tested in 5-KTC-17.5) had on properties was less than that of GTC; how- ever, relative to ATC, it too had higher %Elo and lower TS. Both of the cations in these salts were to the right of ammonium in the Hofmeister series. Magnesium was to the right as well; however, MTC (tested as 7-MTC-17.5) had lower %Elo and higher TS than ATC. As previously mentioned, the Hofmeister series was devel- oped to predict properties in water solution, and so its applicabil- ity may be different here. MTC has a cation with a different charge (+2), which may be a factor when defining the impact cations have on physical properties.
Effect of Relative Humidity—ATC Although the effect that ATC has on physical properties, such as %Elo and the Tg of the zein article containing ATC (discussed earlier), suggest that ATC is a plasticizer of zein, for the increased elongation to be observed some amount of water must be present. Shown in Table IV are the physical properties of select formula- Fig. 7. Predicted tensile strength (TS) of various ammonium thiocyanate tions at different relative humidities. For the control (C17.5), as (ATC) formulations versus actual TS using the following equation: TS = the relative humidity increased, %Elo and toughness increased 32.85 + (–1.23 × %TEG) + (–1.08 × %ATC) + (–0.04 × %TEG × and TS and YM decreased. For the salts, at the lowest relative %ATC). Bold line represents fitted equation, and thin line represents ideal humidity tested the %Elo was less than or equal to the control, relationship of predicted TS = actual TS. TEG = tri(ethylene glycol). suggesting that the thiocyanate salts were not efficient traditional
TABLE IV Impact of % Relative Humidity on Physical Properties of Zein Films Having 17.5% TEG with Various Thiocyanate Saltsa % Relative TS %Elo YM Toughness Formulation Humidity % Moisture TS (St. Dev.) %Elo (St. Dev.) YM (St. Dev.) Toughness (St. Dev.) C17.5 15 3.2 25.2 0.2 10 1.1 447 20 1.4 0.1 C17.5 50 6.0 10.2 0.7 52 12 120 11 2.9 0.3 C17.5 70 10.4 3.7 0.6 328 24 21.7 12.3 9.7 2.2 4-ATC-17.5 15 2.2 19.8 2.2 7 0.3 334 39 0.7 0.1 4-ATC-17.5 50 5.6 1.6 0.1 499 54 7 1 7.1 0.7 4-ATC-17.5 70 8.3 1.1 0.2 648 2 0.9 0.4 4.5 0.6 6-GTC-17.5 15 4.1 18.1 1.2 9 0.6 283 20 0.8 0.1 6-GTC-17.5 50 5.8 0.8 0.1 1,203 91 2 0 7.3 1.2 6-GTC-17.5 70 11.0 0.7 0.1 865 40 0.4 0.1 4.2 0.4 5-KTC-17.5 15 1.7 17.5 1.5 7 0.4 303 17 0.6 0.1 5-KTC-17.5 50 6.1 1.1 0.0 879 11 9 6 6.6 0.7 5-KTC-17.5 70 9.0 0.3 0.0 1,738 5 0.2 0.1 3.1 0.2 7-MTC-17.5 15 2.9 22.3 1.2 5 0.6 512 22 0.5 0.1 7-MTC-17.5 50 7.1 2.2 0.4 399 56 13 4 8.2 1.7 7-MTC-17.5 70 9.2 0.2 0.1 985 117 0.9 0.5 1.7 0.7 a TEG = tri(ethylene glycol); TS = tensile strength; %Elo = elongation to break; YM = Young’s modulus; ATC = ammonium thiocyanate; GTC = guanidine thio- cyanate; KTC = potassium thiocyanate; and MTC = magnesium thiocyanate.
Vol. 90, No. 3, 2013 209 plasticizers. However, as the relative humidity increased, the U.S. patent 2413501. %Elo increased and TS decreased quickly. Water was necessary James, A. L. 1945. Zein dispersions. U.S. patent 2377237. for these salts to affect the physical properties of zein. This effect Jenkins, H. S., and Magee, J. R. 1958. Manufacture of protein fibers. U.S. was independent of the cation chosen. Water is a known plasti- patent 2845362. cizer for zein (Lawton 2004; Selling et al 2004), and as a plasti- Jiang, Q., and Yang, Y. 2011. Water-stable electrospun zein fibers for potential drug delivery. J. Biomat. Sci. Poly. Ed. 22:1393-1408. cizer, it will increase the free volume within the protein. Appar- Lawton, J. W. 2002. Zein: A history of processing and use. Cereal Chem. ently, increased free volume must be present for the salts to affect 79:1-18. the physical properties of zein. The large changes in properties Lawton, J. W. 2004. Plasticizers for zein: Their effect on tensile prop- with changes in humidity may have value in certain end uses such erties and water absorption of zein films. Cereal Chem. 81:1-5. as humidity sensors. Padua, G. W., and Santosa, F. X. B. 1999. Tensile properties and water absorption of zein sheets plasticized with oleic and linoleic acids. J. CONCLUSIONS Agric. Food Chem. 47:2070-2074. Paraman, I., and Lamsal, B. P. 2011. Recovery and characterization of α A new class of plasticizer for zein was developed using non- -zein from corn fermentation coproducts. J. Agric. Food Chem. 59:3071-3077. volatile thiocyanate salts. It was found that ATC, KTC, and GTC Paramawati, R., Yoshino, T., and Isobe, S. 2001. Properties of plasticized- salts can be used to increase the elongation and reduce the modu- zein film as affected by plasticizer treatments. Food Sci. Technol. Res. lus of zein films. Toughness also increased in these formulations 7:191-194. that included ATC. The salts required the use of TEG and moder- Park, S. K., Rhee, C. O., Bae, D. H., and Hettiarachchy, N. S. 2001. Me- ate humidity to increase elongation. At low humidity the film chanical properties and water-vapor permeability of soy-protein films samples were brittle, and at high humidity the samples were so affected by calcium salts and glucono-δ-lactone. J. Agric. Food Chem. weak that they would fail at only moderately higher elongation. 49:2308-2312. Thiocyanate salts were shown to interact with the zein proteins in Reddy, N., Li, Y., and Yang, Y. 2009. Alkali-catalyzed low temperature solution. Additional studies are in progress examining the effects wet crosslinking of plant proteins using carboxylic acids. Biotechnol. Prog. 25:139-146. of other anions and cations and how they affect the properties Rembert, K. B., Paterová, J., Heyda, J., Hilty, C., Jungwirth, P., and detailed in this study. Cremer, P. S. 2012. Molecular mechanisms of ion-specific effects on proteins. J. Am. Chem. Soc. 134:10039-10046. ACKNOWLEDGMENTS Santosa, F. X. B., and Padua, G. W. 2000. Thermal behavior of zein sheets plasticized with oleic acid. Cereal Chem. 77:459-462. A. J. Thomas is thanked for performing the rheological studies on Selling, G. W., Sessa, D. J., and Palmquist, D. E. 2004. Effect of water solutions and films. Karl Vermillion is thanked for performing the NMR and tri(ethylene) glycol on the rheological properties of zein. Polymer analyses. 45:4249-4255. Selling, G. W., Woods, K. K., and Biswas, A. 2012. Electrospun zein LITERATURE CITED fibers using glyoxal as the crosslinking reagent. J. Appl. Poly. Sci. 123:2651-2661. Baldwin, R. L. 1996. How Hofmeister ion interactions affect protein Sessa, D. J., Mohamed, A., and Byars, J. A. 2008. Chemistry and physical stability. Biophysical J. 71:2056-2063. properties of melt-processed and solution-cross-linked corn zein. J. Cho, Y., Zhang, Y., Christensen, T., Sagle, L. B., Chilkoti, A., and Cremer, Agric. Food Chem. 56:7067-7075. P. S. 2008. Effects of Hofmeister anions on the phase transition tem- Seymour, R. B., and Carraher, C. E. 1992. Rheology and solubility. Pages perature of elastin-like polypeptides. J. Phys. Chem. B 112:13765- 61-70 in: Polymer Chemistry: An Introduction, 3rd Ed. Marcel Dekker: 13771. New York. Cline, E. T. 1949. Continuous spinning and stretching of zein filaments. Shashkina, J. A., Philippova, O. E., Zaroslov, Y. D., Khokhlov, A. R., U.S. patent 2475879. Pryakhina, T. A., and Blagodatskikh, I. V. 2005. Rheology of viscoelas- Croston, C. B., and Evans, C. D. 1949. Method of producing prolamine tic solutions of cationic surfactant. Effect of added associating poly- filaments. U.S. patent 2478248. mer. Langmuir 21:1524-1530. Croston, C. B., Evans, C. D., and Smith, A. K. 1945. Zein fibers—Prepa- Silverstein, R. M., Bassler, G. C., and Morrill, T. C. 1981. Proton NMR. ration by wet spinning. J. Ind. Eng. Chem. (Washington, D.C.) Page 220 in: Spectrometric Identification of Organic Compounds. 37:1194-1198. Wiley: New York. Evans, C. D., and Croston, C. B. 1949. Formaldehyde curing of zein Swallen, L. C. 1939. Zein filaments. U.S. patent 2156929. fibers. Textile Res. J. 19:202-211. Tamiola, K., and Mulder, F. A. A. 2012. Using NMR chemical shifts to Gao, C., Stading, M., Wellner, N., Parker, M. L., Noel, T. R., Mills, E. N. C., calculate the propensity for structural order and disorder in proteins. and Belton, P. S. 2006. Plasticization of a protein-based film by glyc- Biochem. Soc. Trans. 40:1014-1020. erol: A spectroscopic, mechanical, and thermal study. J. Agric. Food Whitford, D. 2005. Protein expression, purification and characterization. Chem. 54:4611-4616. Pages 325-326 in: Proteins: Structure and Function. Wiley: Hoboken, NJ. Ghanbarzadeh, B., Oromiehie, A. R., Musavi, M., Falcone, P. M., Jomeh, Wu, L., Wen, Q., and Yang, X. 2010. Effect of plasticizer on surface and Z. E., and Rad, E. R. 2007. Study of mechanical properties, oxygen mechanical properties of zein films. Huagong Xuebao/CIESC J. 61:137- permeability and AFM topography of zein films plasticized by polyols. 145. Packaging Technol. Sci. 20:155-163. Wu, Q., Sakabe, H., and Isobe, S. 2003. Studies on the toughness and Gillgren, T., and Stading, M. 2008. Mechanical and barrier properties of water resistance of zein-based polymers by modification. Polymer avenin, kafirin, and zein films. Food Biophys. 3:287-294. 44:3901-3908. Gillgren, T., Barker, S. A., Belton, P. S., Georget, D. M. R., and Stading, Yao, C., Li, X., and Song, T. 2007. Electrospinning and crosslinking of M. 2009. Plasticization of zein: A thermomechanical, FTIR, and die- zein nanofiber mats. J. Appl. Poly. Sci. 103:380-385. lectric study. Biomacromolecules 10:1135-1139. Zinoviadou, K. G., Koutsoumanis, K. P., and Biliaderis, C. G. 2010. Heuvingh, J., Zappa, M., and Fery, A. 2005. Salt softening of polyelectro- Physical and thermo-mechanical properties of whey protein isolate lyte multilayer capsules. Langmuir 21:3165-3171. films containing antimicrobials, and their effect against spoilage flora Huppert, O. 1946. Artificial fibers from globular and fibrous proteins. of fresh beef. Food Hydrocolloids 24:49-59.
[Received September 28, 2012. Accepted January 15, 2013.]
210 CEREAL CHEMISTRY